Please click on the photo below to see more photos of this specie
5/4 S2S1E KD - $ 5.52 BF
12/4 KD $ 7.92 BF
Bowl Blanks available, Please inquire.
Smells most excellent - assuming you are not allergic to it
Assumed, Wood Working Properties & Specifications
Other Common Names: Cedro (Central and South America), Acajou rouge (French West Indies), Cedre rouge (French Guiana), Ceder (Surinam).
Distribution: Cedrela occurs from Mexico to Argentina and is found in all countries except Chile. Trees make their best growth on rich, well-drained humid sites but may also compete favorably on drier hillsides; intolerant of water- logged locations.
The Tree: Under favorable conditions will reach heights over 100 ft and diameters 3 to 6 ft above the substantial buttresses. Straight cylindrical boles clear for 40 to 60 ft.
General Characteristics: Heartwood pinkish- to reddish brown when freshly cut, becoming red or dark reddish brown, sometimes with a purplish tinge, after exposure; sharply to rather poorly demarcated from the pinkish to white sapwood. Grain usually straight, sometimes interlocked; texture rather fine and uniform to coarse and uneven; luster medium to high and golden; distinctive cedary odor usually pronounced, some specimens with bitter taste.
Weight: Basic specific gravity (ovendry weight/green volume) very variable ranging from 0.30 to 0.60, averaging about 0.40; air-dry density ranges from 23 to 47 pcf, averaging about 30 pcf.
Mechanical Properties: (First set of data based on 2-in. standard;
second set 2- cm standard.)
Moisture content Bending strength Modulus of elasticity Maximum crushing strength
(%) (Psi) (1,000 psi) (Psi)
Green (74) 7,510 1,310 3,370
12% 11,530 1,440 6,210
Green (30) 9,100 1,200 4,080
15% 11,750 NA 5,650
Janka side hardness about 550 lb for green material and 600 lb for air dry. Forest Products Laboratory toughness average for green and dry material 106 in.- lb (5/8-in specimen).
Drying and Shrinkage: Easy to air-season or kiln-dry, slight warp with little or no checking. Kiln schedule T10-D4S is suggested for 4/4 stock and T8-D3S for 8/4. A 200o F heating for 8 to 17 hours at a relative humidity of 60 percent is suggested to control oil and gum exudates in service. Shrinkage green to ovendry: radial 4.2%; tangential 6.3%; volumetric 10.3%. Movement in service rated as small.
Working Properties: Cedro is easy to work with hand and machine tools but somewhat difficult to bore cleanly. Easy to cut into veneer but with some tendency for wooly surfaces to occur; good nailing and gluing properties; stains and finishes well but gums and oils sometimes are a problem in polishing.
Durability: Heartwood is rated as durable but there is some variability within species; resistant to both subterranean and dry-wood termites. Low resistance to attack by marine borers. Wood has excellent weathering characteristics.
Preservation: Heartwood is reported to be extremely resistant to preservation treatments. Reports on treatability of sapwood are conflicting.
Uses: Wood is favored for millwork, cabinets, fine furniture,
musical instruments, boat building, patterns, sliced- and rotary-cut veneer,
decorative and utility plywoods, cigar wrappers, and cigar boxes. Volatile
oils may restrict use for some applications (e.g., clock cases).
Prices and inventory listed are subject
to change without notice.
Please contact us for up to the minute pricing and
inventory, before quoting jobs from this site.
Please close this window when done to continue with navigation of our site.
If a search engine or link brought you to this page,
this Return Home button to get to our starting / Main page.
Otherwise just close
this window to return to the main menu screen.
Try our mirror site if this connection is slow for you.